| ||Format||Pages||Price|| |
|8||$44.00||  ADD TO CART|
|Hardcopy (shipping and handling)||8||$44.00||  ADD TO CART|
|Standard + Redline PDF Bundle||16||$52.80||  ADD TO CART|
This specification establishes the requirements for electrodeposited gold coatings for engineering applications, employed specifically for their corrosion and tarnish resistance (including resistance to fretting corrosion and catalytic polymerization), bondability, low and stable contact resistance, solderability, and infrared reflectivity. This specification does not cover gold coatings produced from autocatalytic, immersion, and vapor deposition. Coatings shall be classified into types, which characterize minimum purity, and codes, which designate Knoop hardness. Coatings shall be sampled, tested and conform to specified requirements as to purity, hardness, appearance, thickness, mass per unit area, ductility, adhesion (assessed by either bend, heat, or cutting test), and integrity (including gross defects, mechanical damage, and porosity).
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers requirements for electrodeposited gold coatings that contain not less than 99.00 mass % gold and that are used for engineering applications.
1.2 Specifically excluded from this specification are autocatalytic, immersion, and vapor deposited gold coatings.
1.3 Gold coatings conforming to this specification are employed for their corrosion and tarnish resistance (including resistance to fretting corrosion and catalytic polymerization), bondability, low and stable contact resistance, solderability, and infrared reflectivity. Several types of coatings, differing in gold purity and hardness, are covered by this specification.
1.4 The values stated in SI units are to be regarded as the standard. Values provided in parentheses are for information only.
1.5 The following hazards caveat pertains only to the test methods section, Section 9, of this specification: This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B183 Practice for Preparation of Low-Carbon Steel for Electroplating
B242 Guide for Preparation of High-Carbon Steel for Electroplating
B253 Guide for Preparation of Aluminum Alloys for Electroplating
B254 Practice for Preparation of and Electroplating on Stainless Steel
B281 Practice for Preparation of Copper and Copper-Base Alloys for Electroplating and Conversion Coatings
B322 Guide for Cleaning Metals Prior to Electroplating
B343 Practice for Preparation of Nickel for Electroplating with Nickel
B374 Terminology Relating to Electroplating
B481 Practice for Preparation of Titanium and Titanium Alloys for Electroplating
B482 Practice for Preparation of Tungsten and Tungsten Alloys for Electroplating
B487 Test Method for Measurement of Metal and Oxide Coating Thickness by Microscopical Examination of Cross Section
B489 Practice for Bend Test for Ductility of Electrodeposited and Autocatalytically Deposited Metal Coatings on Metals
B499 Test Method for Measurement of Coating Thicknesses by the Magnetic Method: Nonmagnetic Coatings on Magnetic Basis Metals
B504 Test Method for Measurement of Thickness of Metallic Coatings by the Coulometric Method
B507 Practice for Design of Articles to Be Electroplated on Racks
B542 Terminology Relating to Electrical Contacts and Their Use
B558 Practice for Preparation of Nickel Alloys for Electroplating
B567 Test Method for Measurement of Coating Thickness by the Beta Backscatter Method
B568 Test Method for Measurement of Coating Thickness by X-Ray Spectrometry
B571 Practice for Qualitative Adhesion Testing of Metallic Coatings
B578 Test Method for Microhardness of Electroplated Coatings
B602 Test Method for Attribute Sampling of Metallic and Inorganic Coatings
B678 Test Method for Solderability of Metallic-Coated Products
B697 Guide for Selection of Sampling Plans for Inspection of Electrodeposited Metallic and Inorganic Coatings
B735 Test Method for Porosity in Gold Coatings on Metal Substrates by Nitric Acid Vapor
B741 Test Method for Porosity In Gold Coatings On Metal Substrates By Paper Electrography
B748 Test Method for Measurement of Thickness of Metallic Coatings by Measurement of Cross Section with a Scanning Electron Microscope
B762 Test Method of Variables Sampling of Metallic and Inorganic Coatings
B765 Guide for Selection of Porosity and Gross Defect Tests for Electrodeposits and Related Metallic Coatings
B799 Test Method for Porosity in Gold and Palladium Coatings by Sulfurous Acid/Sulfur-Dioxide Vapor
B809 Test Method for Porosity in Metallic Coatings by Humid Sulfur Vapor (Flowers-of-Sulfur)
D1125 Test Methods for Electrical Conductivity and Resistivity of Water
D3951 Practice for Commercial Packaging
F390 Test Method for Sheet Resistance of Thin Metallic Films With a Collinear Four-Probe Array
ICS Number Code 25.220.40 (Metallic coatings)
UNSPSC Code 11101801(Gold)
ASTM B488-11, Standard Specification for Electrodeposited Coatings of Gold for Engineering Uses, ASTM International, West Conshohocken, PA, 2011, www.astm.orgBack to Top